Ambipolar Surface State Thermoelectric Power of Topological Insulator Bi2Se3 Dohun Kim,† Paul Syers,† Nicholas P. Butch,‡ Johnpierre Paglione,† and Michael S. Fuhrer*,†,§ †

Center for Nanophysics and Advanced Materials, Department of Physics, University of Maryland, College Park, Maryland 20742-4111, United States ‡ Center for Neutron Research, National Institute of Standards and Technology, Gaithersburg, Maryland 20899-6102, United States § School of Physics, Monash University, 3800 Victoria, Australia S Supporting Information *

ABSTRACT: We measure gate-tuned thermoelectric power of mechanically exfoliated Bi2Se3 thin ﬁlms in the topological insulator regime. The sign of the thermoelectric power changes across the charge neutrality point as the majority carrier type switches from electron to hole, consistent with the ambipolar electric ﬁeld eﬀect observed in conductivity and Hall eﬀect measurements. Near the charge neutrality point and at low temperatures, the gate-dependent thermoelectric power follows the semiclassical Mott relation using the expected surface state density of states but is larger than expected at high electron doping, possibly reﬂecting a large density of states in the bulk gap. The thermoelectric power factor shows signiﬁcant enhancement near the electron−hole puddle carrier density ∼0.5 × 1012 cm−2 per surface at all temperatures. Together with the expected reduction of lattice thermal conductivity in low-dimensional structures, the results demonstrate that nanostructuring and Fermi level tuning of three-dimensional topological insulators can be promising routes to realize eﬃcient thermoelectric devices. KEYWORDS: Topological insulators, thermoelectric power, ambipolar electric ﬁeld eﬀect, bismuth selenide, charge transfer doping

T

Although there have been theoretical investigations of thermal and thermoelectric properties of Dirac materials including graphene and TIs6,7,11−15 and thermoelectric transport in carbon nanotubes16 and graphene9,17−19 have been studied experimentally, it has been diﬃcult to experimentally observe clear surface thermoelectric transport in TI materials due to the high level of bulk doping present in as-grown TI crystals.20,21 Here, we experimentally demonstrate the ﬁrst measurement of thermoelectric power of topological insulator Bi2 Se3 dominated by metallic surface states. We show a clear ambipolar electric ﬁeld eﬀect indicated by the sign change of the thermoelectric power across the charge neutrality point where the charge transport exhibits minimum conductivity. We ﬁnd that the gate-dependent thermoelectric power exhibits an agreement with the semiclassical Mott relation10 consistent with surface band structure, however, we also ﬁnd deviation with expected surface-dominated thermoelectric power at high electron doping voltage where bulk states are likely populated. We also demonstrate signiﬁcant (up to 2-fold) enhancement of the power factor σS2 for a Dirac band as the Fermi energy approaches the Dirac point, indicating that surface state

he eﬃciency of thermoelectric devices is determined by the thermoelectric ﬁgure of merit ZT = σS2T/κ, where S is thermoelectric power (Seebeck coeﬃcient) and σ and κ are electrical and thermal conductivity respectively. For a given thermal conductivity (typically dominated by phonons) and temperature, ZT is determined by the electronic structure of a material through the power factor σS2. Nanostructuring has long been seen as a promising route to increase ZT both through decreasing κ via phonon boundary scattering, and increasing the power factor through conﬁnement-induced band structure eﬀects.1 The discovery that important thermoelectric materials Bi1−xSbx and Bi2(Se,Te)32−4 are in fact threedimensional (3D) topological insulators (TI) has triggered new directions to improve ZT via nanostructuring. The 3D TIs have an insulating bulk but metallic surface states with spinmomentum helicity that cannot be localized by nonmagnetic disorder.4,5 Recent theoretical calculations6,7 show that signiﬁcant enhancement of ZT is expected in 3D TIs particularly in thin ﬁlm geometry where top and bottom surfaces can hybridize and form a surface gap.8 Thermoelectric power is also of great interest in understanding the electronic transport properties of Dirac electronic systems,9 thus measurement of the thermoelectric properties of TI surface states can elucidate details of the electronic structure of the ambipolar nature of topological metallic surface states that cannot be probed by conductance measurements alone.10 © 2014 American Chemical Society

Received: August 27, 2013 Revised: February 28, 2014 Published: March 7, 2014 1701

dx.doi.org/10.1021/nl4032154 | Nano Lett. 2014, 14, 1701−1706

Nano Letters

Letter

temperature of 10 K with the highest Hall mobility at low temperature of ∼1100 cm2/(V s). The slope nH versus Vg reﬂects the expected capacitance of ∼11 nF cm−2 for the 300 nm SiO2 gate dielectric. At T = 10 K, the device shows clear ambipolar electric ﬁeld eﬀect which is indicated by minimum conductivity σmin at charge neutrality point VD ∼ −50 V and corresponding sign change of Hall carrier density nH (see Figure 1a, inset) consistent with the gapless Dirac band structure of topological surface states.22 As it was shown previously,22−24 σ is linearly proportional to Vg near VD suggesting that charged impurity scattering limits electronic transport for the present devices.22 The observation of sublinear σ(Vg) at Vg further away from VD may indicate that there are additional types of disorder, for example, neutral point defects, which need to be considered,25 though as discussed further below it may also reﬂect the population of lowerconductivity bulk states, most likely by ﬁlling in-gap impurity bands. At low temperatures T < 150 K, we observe a change in sign of S, which indicates the sign of the majority charge carrier from positive to negative as Vg crosses VD, consistent with the change in sign of nH. At temperatures starting from about 70 K, thermal population of hole and electron carriers between the bulk valence band and the surface state bands becomes important,26 resulting in a shift of VD to negative voltage, reﬂected also in a shift to negative voltage of the zeroes in S. This thermal activation eﬀect was explained by us in detail in a previous work.26 At higher temperatures T ≥ 150 K, thermal activation is signiﬁcant enough that the sign change cannot be observed within the range of accessible Vg. The electron−hole asymmetry observed in both σ and S is consistent with the asymmetric surface band structure of Bi2Se3.3,27 The peak value of S reaches ∼170 μV/K at 240 K in the majority of devices measured. We now turn to a quantitative analysis of gate-tuned surface state thermopower in the TI regime. For semiclassical transport the carrier-density dependence of the thermopower is described by the Mott relation10

conduction in TI materials is a promising route to thermopower enhancement, even in the absence of a hybridization gap.6,7 We also discuss possible routes for further enhancement to the limit predicted theoretically.6,7 We study mechanically exfoliated Bi2Se3 single crystals20 with thickness approximately 13 ± 1 nm, which is conﬁrmed using atomic force microscopy (AFM). We use a thermopower measurement technique using microfabricated heaters and thermistors, previously developed and used to study thermoelectric properties of carbon nanotubes16 and graphene9,18,19 (see also Methods for description of measurement scheme). As described previously,22 we employed molecular charge transfer p-type doping by thermal evaporation of 2,3,5,6-tetraﬂuoro7,7,8,8-tetracyanoquinodimethane to reduce the high level of ntype doping. Further tuning of carrier density is accomplished using a Si back gate and 300 nm SiO2 gate dielectric. We showed previously22 that in such thin Bi2Se3 slabs in the TI regime that the top and bottom surfaces are strongly capacitively coupled through the high-dielectric-constant bulk20 (ε ∼100) and couple nearly equally to the back gate. Figure 1a,b shows sheet conductivity σ and thermopower S respectively as a function of back gate voltage Vg for a representative Bi2Se3 device for several temperatures T from 10 to 240 K. We measure Hall carrier density nH about 3 × 1012 cm−2 at zero gate voltage (see Figure 1a, inset) at the

S=−

π 2kB2T d ln σ 3e dE F

=−

π 2kB2T 1 dσ dVg 3e σ dVg dE F

=−

π 2kB2T 1 dσ D(Vg) 3e σ dn

(1)

where e is the elementary charge, n = Cg(Vg − VD)/e is gate induced carrier density with gate capacitance Cg ≈ 11.1 nFcm−2, kB is the Boltzmann constant, EF is Fermi energy, and D(Vg) is the gate-voltage-dependent density of states. The ﬁrst equality can be tested with concurrently measured σ(Vg) along with the expected band structure and has been shown to provide a good description of S(Vg) in mesoscopic carbon nanotube16 and graphene9,17,18 ﬁeld-eﬀect devices. For a Dirac material with Coulomb scattering, eq 1 predicts a divergence in S ∼ (Vg − VD)−1/2, since σ ∼ (Vg − VD) and EF ∼ (Vg − VD)1/2.9,15 This enhancement is the essence of the enhanced thermopower expected for Dirac surface states. The divergence is cut oﬀ by the electron−hole puddle carrier density n*; we can estimate n* ∼ 0.5 × 1012 cm−2 per surface from the minimum in nH (see Figure 1a, inset). For a detailed comparison with eq 1, we ﬁrst compare the measured S with predicted S (SMott) using the known surface

Figure 1. (a) The 2D conductivity σ as a function of back gate voltage Vg of a ∼13 nm thick Bi2Se3 measured at temperatures indicated in the caption. The inset shows Hall carrier density nH simultaneously measured with σ at the temperature of 10 K. (b) Thermopower S as a function of Vg measured at the same condition as in (a) showing ambipolar electric ﬁeld eﬀect consistent with corresponding σ measurement. The inset shows optical micrograph of the device. The scale bar is 2 μm.. 1702

dx.doi.org/10.1021/nl4032154 | Nano Lett. 2014, 14, 1701−1706

Nano Letters

Letter

Figure 2. (a) Experimentally measured thermopower S (black solid curve) and thermopower estimated from the Mott relation SMott including eﬀect of thermal activation of carriers from bulk valence band and shift of Dirac point (see main text for discussion) as a function of Vg at the temperatures from 10 to 240 K. Dashed horizontal lines denote zeros of thermopower. Shaded areas show gate voltage regions where thermal activation of bulk carriers is signiﬁcant. (b) Calculated surface (black curves) and bulk (blue curves) carrier densities as a function of Vg at the same temperatures as in (a) using band model described in the main text.

band structure of Bi2Se3.3,27 We calculate the factor dVg/dEF numerically using a band model as developed previously26 using the surface band with dispersion E2D(k) = ℏvF,0k + (ℏ2k2/2m*s ). For the calculation, we used the parameters of the Fermi velocity near Dirac point vF,0 = 3 × 107 cm/s, and eﬀective mass ms* = 0.3 me of the surface band that are reasonable for Bi2Se3 from the ARPES measurements.3,27 We also calculated expected carrier density using surface band and bulk valence and conduction bands. For the bulk band density of states we used ﬁrst principles calculation of bulk Bi2Se3 reported elsewhere.28 Figure 2a shows a detailed comparison of the measured thermopower (S, black solid) and calculated surface state thermopower from semiclassical Mott relation (SMott, red solid) using conductivity data and band model described above for various temperatures from 10 to 240 K. We ﬁnd a good agreement at low temperature (for example, 10 K) and near charge neutrality point, as expected for degenerate electrons in the metallic surface band where the entropy transported in the channel is proportional to the number of thermally activated carriers over the degenerate Fermi sea (S ∼ T/EF).9 This agreement is also true near VD due to charge inhomogeneity driven puddle density >1012 cm−2, which renders the system to remain in the degenerate regime. We observe a peak in S at a gate voltage roughly corresponding to the electron−hole puddle carrier density n*, below which the value of S decreases due to cancellation of n-type and p-type thermopowers with a magnitude which can be explained by the Mott relation [eq 1], as observed previously for graphene.9 The Mott relation also reproduces the position and magnitude of some of the ﬁne features in the low-temperature (10 and 20 K) gate-voltage

dependent thermopower (presumably due to universal conductance ﬂuctuations). Figure 2b shows calculated surface (black curves) and bulk (blue curves) carrier densities at given total charge density ﬁxed by Vg as a function of Vg at the same temperatures in Figure 2a. We observe signiﬁcant thermal activation at the temperatures T ≥ 150 K near or below −50 V (Figure 2b shaded area) as explored in detail previously.26 However, for positive Vg up to Vg = 80 V, thermal activation to the bulk conduction band is negligible at all temperatures. We also observe an additional enhancement of the thermopower which is not predicted by the Mott relation assuming only surface states. This can be seen especially at high positive Vg and high temperature where SMott tends to zero but the measured S saturates to a constant. The ratio S/SMott is as large as 7 at T = 240 K and Vg = +80 V. Figure 3a,b shows the temperature dependence of the measured S and predicted SMott at ﬁxed Vg ranging −80 < Vg < 80 V indicated in the caption, and Figure 3c shows the additional thermopower S − SMott. The additional thermopower is negative with magnitude increasing monotonically with temperature and roughly independent of gate voltage. Phonon drag is a known contribution to thermopower beyond eq 1. However, the phonon drag contribution to the thermopower Sp in a Dirac electronic system was found to obey Herring’s law Sp = −vsΛ/μpT where vs is the sound velocity, Λ is the phonon mean free path, and μp is the phonon-limited carrier mobility.29 We expect at high temperature Λ ∼ 1/T, μp ∼ 1/nT,26 and thus Sp ∼ n/T, in sharp contrast to the experimental observation of additional thermopower independent of n and increasing with T (roughly proportional to T2 at high T). Similarly, temperature-dependent screening gives corrections to the conductivity and thermo1703

dx.doi.org/10.1021/nl4032154 | Nano Lett. 2014, 14, 1701−1706

Nano Letters

Letter

Figure 4. Density of states D estimated from Mott relation (eq 1) as a function of gate voltage Vg at temperatures indicated in the caption. Dashed red (dash-dot purple) curves show expected surface (bulk) density of states of Bi2Se3.

enhancement of D is seen in the conduction band at low temperatures, well below the expected onset of the bulk conduction band density of states at Vg > 80 V. This possibly reﬂects a large smearing of the conduction band edge or the presence of a high density of impurity states in the bulk gap that are not reﬂected in the carrier density calculation in Figure 2b. We note that the extraction of D using the Mott relation does not determine whether the states are conducting or insulating. However, Hall carrier density measurements suggest that the vast majority of the gate-induced charge is delocalized. If bulk states contribute to the conduction at large electron doping, this could provide an alternative explanation for the sublinearity of σ(Vg) observed in the same regime. On raising the temperature, we observe a ﬁlling-in of the dip in D associated with the Dirac point. This is qualitatively consistent with thermal smearing. The larger D implies that our gate voltage window accesses a smaller Fermi energy range, therefore larger thermal activation eﬀects are expected. This would also explain the unexpected supralinear S(T) seen in Figure 3. While the presence of an unexpectedly large D inside the bulk gap qualitatively explains the observed features of the data, a quantitative understanding will require a more detailed knowledge of the origin of such states. Particularly if the states are inhomogeneously distributed through the sample due to screening of disorder or “puddling” or due to band-bending then the extraction of D is only qualitative. We conclude that the thermopower very close to the Dirac point and at low temperature is explained well by the expected D and measured σ(Vg) of the surface states alone. Away from the Dirac point, and at higher temperature, deviations are observed that are presumed to be due to additional states in the bulk band gap along with increased thermal activation to these states. We ﬁnally turn to discuss enhanced thermoelectric eﬃciency in the TI regime. A simple analysis for the Dirac surface state predicts S ∼ (Vg − VD)−1/2, σ ∼ (Vg − VD) hence power factor σS2 is independent of Vg. In recent theoretical studies,6,7 a large enhancement of the power factor is predicted at low Fermi energies when considering thin slabs of Bi2Se3 and Bi2Te3 in which intersurface hybridization induces a surface gap, but no enhancement of the power factor is predicted for ungapped surface states near the Dirac point.6 Figure 5 shows the measured σS2 as a function of Vg at temperatures from 20 to 240 K. Notably, a clear enhancement of σS2 can be observed near Vg = −40 V at all temperatures, which corresponds to

Figure 3. Variation of the (a) measured thermopower S and (b) predicted thermopower SMott at ﬁxed Vg ranging −80 < Vg < 80 V indicated in the caption as a function of temperature from 10 to 240 K showing nonlinear and nonmonotonic temperature dependence. (c) S − SMott as a function of temperature at the same Vg given in a and b.

power proportional to (kBT/EF)2;15 such corrections should be unimportant at high Vg,26 and moreover no strong dependence on EF or Vg is seen. By measuring an additional sample with factor of 3 smaller contact area we found quantitatively similar temperature-dependent thermopower (within 5 μV/K), indicating that the eﬀect of contact barrier on the additional contribution to the measured thermopower is small (see Supporting Information). In the Supporting Information, we also show the negligible temperature dependence of the carrier density in the electron-doped regime for a similarly prepared sample, which precludes temperature dependent charge transfer as the source of additional contribution to the thermopower. We expect that the Mott formula is a good approximation for temperatures kBT < EF. Because of electron−hole puddling the eﬀective Fermi energy is never signiﬁcantly smaller than 50 meV, and we expect this approximation to be reasonable for the temperature range studied. Furthermore the approximation holds for multiband systems, and the Mott relation (second equality in eq 1) can be inverted using the measured S and σ(Vg) to obtain a total density of states D. Figure 4 shows a comparison of the experimentally obtained gate-dependent density of states from inversion of the Mott formula at various temperatures (solid lines) with the expected surface3,27 (dashed lines) and bulk28 (dash-dot lines) densities of states with bulk valence band edge Ev ≈ −60 meV respect to the Dirac point.3,26,27 Near charge neutrality point of ∼−50 V and at low temperatures, the measured D agrees well with expected surface density of states for Bi2Se3 as expected, reﬂecting the agreement seen in Figure 2. Away from charge neutrality point, a large 1704

dx.doi.org/10.1021/nl4032154 | Nano Lett. 2014, 14, 1701−1706

Nano Letters

Letter

with bulk resistivity exceeding 2 mΩcm at 300 K were grown by melting high purity bismuth (6N) and selenium (5N) in sealed quartz ampules.20 The crystals were exfoliated with Scotch tape and deposited on doped Si covered with 300 nm SiO2. Thin Bi2Se3 crystals with thickness in the order of ∼10 nm were identiﬁed by combined use of optical and atomic force microscopy (AFM). Electron beam lithography, thermal evaporation and liftoﬀ techniques were used to make electrical contact, thermistors and external heaters (Cr/Au: 5/70 nm). Typical line widths of thermistors were restricted to be less than 500 nm to ensure local thermometry. Thin ﬁlms were patterned into Hall bar geometry (see Figure 1b, inset) with typical aspect ratio (L/W) of about 2 and shortest length exceeding 2 μm using Ar plasma at a pressure of ∼6.7 Pa (5 × 10−2 Torr). Molecular charge transfer doping was done by thermal evaporation of ∼10 nm of 2,3,5,6-tetraﬂuoro-7,7,8,8tetracyanoquinodimethane organic molecules (SynQuest Laboratories) on top of the fabricated samples.22,33 Measurement. Thermopower measurement was done using Stanford Research Systems SR830 Lock in ampliﬁers and a commercial cryostat equipped with 9 T superconducting magnet. Low frequency ac (ω < 17 Hz) heater currents was applied to the sample and the resultant 2ω thermoelectric voltage ΔV between two ends of thermistors (see Figure 1b, inset) was detected in the open circuit condition.9,16 Temperature diﬀerence ΔT was measured by measuring temperaturecalibrated four probe resistances of the two gold thermistors (see Figure 1b, inset). Finally thermoelectric power was calculated from S = −ΔV/ΔT. Thermopower of Au leads (∼2 μV/K at 300 K) at a given temperature is expected to be negligible compared to that of Bi2Se3 and was not subtracted from the measured S. Carrier density was tuned through 300 nm thick SiO2 dielectric back gate. To stay in the linear response regime, heater current was adjusted (typically 3 to 8 mA) so that the condition ΔT ≪ T at given temperature is satisﬁed.9 Electronic transport measurements were performed using similar four probe lock-in technique with rms current amplitude of 100 nA applied to the device and measuring ﬁrst harmonic (ω) voltage signals.

Figure 5. Thermoelectric power factor σS2 as a function of Vg at various temperatures indicated in the caption. A factor of 2 enhancement of σS2 is observed near Vg ∼ −40 V corresponding to total carrier density of ∼1 × 1012 cm−2.

carrier density n ∼ 1 × 1012 cm−2 or EF ∼ 40 meV with respect to the Dirac point assuming a linear Dirac band for Bi2Se3. At all temperatures the enhancement of σS2 is about factor of 2 compared to the non-TI regime (bulk conducting). The enhancement near the Dirac point is surprising given that we expect the hybridization gap in our 13 nm thick samples to be negligible (∼10 μeV8). The maximum σS2 of ∼3 μW cm−1 K−2 measured at 240 K is an order of magnitude enhancement compared to the value of ∼0.3 μW cm−1 K−2 at 300 K reported for Bi2Se3 nanoﬂakes (highly conducting bulk) prepared by solvothermal method.30 Admittedly, the absolute value of maximum σS2 for the present samples are less than best reported value ∼18 μW cm−1 K−2 of bulk Bi2Se331 at the same temperature. By controlling doping of exfoliated Bi2Se3 we experimentally conﬁrmed the gapless ambipolar nature of the thermopower that is consistent with the existence of topological metallic surface states. Although more works are needed to quantitatively understand the observed deviation of measured S from the semicalssical Mott relation, we ﬁnd a clear enhancement of σS2 near the Dirac point at all temperatures. Because one additionally expects a reduction in thermal conductivity for thin Bi2Se3 compared to bulk,32 we ﬁnd that nanostructuring and Fermi level control of topological insulators are promising strategies to increase ZT by both increasing the power factor and reducing the thermal conductivity. While the power factor for the Bi2Se3 surface states does not exceed the bulk in our samples, there is signiﬁcant room for improvement; we expect that the enhancement of power factor in thin topological insulators in the topological regime can be improved by increasing surface quality (increase electrical conductivity as well as S by reducing n* and thus more closely approaching the Dirac point). For current samples having thickness ∼13 nm we estimate the hybridization gap is in the order of ∼10 μeV,8 much smaller than charge inhomogeneity driven energy broadening, which limits the thermopower enhancement by a factor of 2. Further thinning of the samples to open a sizable hybridization gap between top and bottom surfaces6,8 as well as further reducing the lattice thermal conductivity32 could produce a larger enhancement of thermoelectric performance. Methods. Bi2Se3 Thermopower Device Fabrication. Lowdoped (carrier density ∼1017 cm−3) bulk Bi2Se3 single crystals

■

ASSOCIATED CONTENT

S Supporting Information *

Thermoelectric measurements on additional sample, reproducibility of additional contribution to thermopower, and F4TCNQ charge doping stability. This material is available free of charge via the Internet at http://pubs.acs.org.

■

AUTHOR INFORMATION

Corresponding Author

*E-mail: [email protected]. Present Address

(D.K.) Department of Physics, University of WisconsinMadison, Madison, Wisconsin 53706, U.S.A. Author Contributions

D.K. fabricated devices, performed the electrical measurements, and analyzed the data with M.S.F. P.S., N.P.B, and J.P. prepared single crystal Bi2Se3 starting material. D.K. and M.S.F. wrote the manuscript with contributions from all authors. Notes

The authors declare no competing ﬁnancial interest. 1705

dx.doi.org/10.1021/nl4032154 | Nano Lett. 2014, 14, 1701−1706

Nano Letters

■

Letter

Oxidation As a Source of Surface Degradation Dactor for Bi2Se3. ACS Nano 2011, 5, 4698−4703. (22) Kim, D.; Cho, S.; Butch, N. P.; Syers, P.; Kirshenbaum, K.; Adam, S.; Paglione, J.; Fuhrer, M. S. Surface conduction of topological Dirac electrons in bulk insulating Bi2Se3. Nat. Phys 2012, 8, 459−463. (23) Chen, J. H.; Jang, C.; Adam, S.; Fuhrer, M. S.; Williams, E. D.; Ishigami, M. Charged-impurity scattering in graphene. Nat. Phys. 2008, 4, 377−381. (24) Adam, S.; Hwang, E. H.; Galitski, V. M.; Das Sarma, S. A selfconsistent theory for graphene transport. Proc. Natl. Acad. Sci. U.S.A. 2007, 104, 18392−18397. (25) Das Sarma, S.; Adam, S.; Hwang, E. H.; Rossi, E. Electronic transport in two-dimensional graphene. Rev. Mod. Phys. 2011, 83, 407−470. (26) Kim, D.; Li, Q.; Syers, P.; Butch, N. P.; Paglione, J.; Das Sarma, S.; Fuhrer, M. S. Intrinsic electron-phonon resistivity of Bi2Se3 in the topological regime. Phys. Rev. Lett. 2012, 109, 166801. (27) Zhu, Z. H.; Levy, G.; Ludbrook, B.; Veenstra, C. N.; Rosen, J. A.; Comin, R.; Wong, D.; Dosanjh, P.; Ubaldini, A.; Syers, P.; Butch, N. P.; Paglione, J.; Elfimov, I. S.; Damascelli, A. Rashba spin-splitting control at the surface of the topological insulator Bi2Se3. Phys. Rev. Lett. 2011, 107, 186405. (28) Luo, X.; Sullivan, M. B.; Quek, S. Y. First-principles investigations of the atomic, electronic, and thermoelectric properties of equilibrium and strained Bi2Se3 and Bi2Te3 including van derWaals interactions. Phys. Rev. B. 2012, 86, 184111. (29) Kubakaddi, S. S. Interaction of massless Dirac electrons with acoustic phonons in graphene at low temperatures. Phys. Rev. B 2009, 79, 075417. (30) Kadel, K.; Kumari, L.; Li, W.; Huang, J.; Provencio, P. Synthesis and thermoelectric properties of Bi2Se3 nanostructures. Nanoscale Res. Lett. 2011, 6, 57. (31) Hor, Y. S.; Richardella, A.; Roushan, P.; Xia, Y.; Checkelsky, J. G.; Yazdani, A.; Hasan, M. Z.; Ong, N. P.; Cava, R. J. p-type Bi2Se3 for topological insulator and low-temperature thermoelectric applications. Phys. Rev. B 2009, 79, 195208. (32) Li, G.; Liang, D.; Qiu, R. L. J.; Gao, X. P. A. Thermal conductivity measurement of individual Bi2Se3 nano-ribbon by selfheating three-omega method. Appl. Phys. Lett. 2013, 102, 043104. (33) Pinto, H.; Jones, R.; Goss, J. P.; Briddon, P. R. p-type doping of graphene with F4-TCNQ. J. Phys: Condens. Matter 2009, 21, 402001.

ACKNOWLEDGMENTS This work was supported by NSF Grant DMR-1105224. Preparation of Bi2Se3 was supported by NSF MRSEC (DMR0520471) and NSF (DMR-0952716). N.P.B. was partially supported by the Center for Nanophysics and Advanced Materials. M.S.F. is supported by an ARC Laureate Fellowship.

■

REFERENCES

(1) Snyder, G. J.; Toberer, E. S. Complex thermoelectric materials. Nat. Mater. 2008, 7, 105−114. (2) Chen, Y. L.; Analytis, J. G.; Chu, J. H.; Liu, Z. K.; Mo, S. K.; Qi, X. L.; Zhang, H. J.; Lu, D. H.; Dai, X.; Fang, Z.; Zhang, S. C.; Fisher, I. R.; Hussain, Z.; Shen, Z. X. Experimental realization of a threedimensional topological insulator, Bi2Te3. Science 2009, 325, 178−181. (3) Zhang, H.; Liu, C. X.; Qi, X. L.; Dai, X.; Fang, Z.; Zhang, S. C.; Zhang. Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface. Nat. Phys. 2009, 5, 438−442. (4) Hsieh, D.; Xia, Y.; Qian, D.; Wray, L.; Dil, J. H.; Meier, F.; Osterwalder, J.; Patthey, L.; Checkelsky, J. G.; Ong, N. P.; Fedorov, A. V.; Lin, H.; Bansil, A.; Grauer, D.; Hor, Y. S.; Cava, R. J.; Hasan, M. Z. A tunable topological insulator in the spin helical Dirac transport regime. Nature 2009, 460, 1101−1105. (5) Fu, L.; Kane, C. L.; Mele, E. J. Topological insulators in three dimensions. Phys. Rev. Lett. 2007, 98, 106803. (6) Ghaemi, P.; Mong, R. S. K.; Moore, J. E. In-plane transport and enhanced thermoelectric performance in thin films of the topological Insulators Bi2Te3 and Bi2Se3. Phys. Rev. Lett. 2010, 105, 166603. (7) Ryuji, T.; Shuichi, M. Thermoelectric transport in topological insulators. Semicond. Sci. Technol. 2012, 27, 124005. (8) Zhang, Y.; He, K.; Chang, C. Z.; Song, C. L.; Wang, L. L.; Chen, X. J.; Jin, F.; Fang, Z.; Dai, X.; Shan, W. Y.; Shen, S. Q.; Niu, Q. Q.; Xia, L.; Zhang, S. C.; Ma, X. C.; Xue, Q. K. Crossover of the threedimensional topological insulator Bi2Se3 to the two-dimensional limit. Nat. Phys. 2010, 6, 584−588. (9) Zuev, Y. M.; Chang, W.; Kim, P. Thermoelectric and magnetothermoelectric transport measurements of graphene. Phys. Rev. Lett. 2009, 102, 096807. (10) Cutler, M.; Mott, N. F. Observation of anderson localization in an electron gas. Phys. Rev. 1969, 181, 1336−1340. (11) Foster, M. S.; Aleiner, I. L. Slow imbalance relaxation and thermoelectric transport in graphene. Phys. Rev. B 2009, 79, 085415. (12) Löfwander, T.; Fogelström, M. Impurity scattering and Mott’s formula in graphene. Phys. Rev. B 2007, 76, 193401. (13) Stauber, T.; Peres, N. M. R.; Guinea, F. Electronic transport in graphene: A semiclassical approach including midgap states. Phys. Rev. B 2007, 76, 205423. (14) Tretiakov, O. A.; Abanov, A.; Sinova, J. Holey topological thermoelectrics. Appl. Phys. Lett. 2011, 99, 113110. (15) Hwang, E. H.; Rossi, E.; Das Sarma, S. Theory of thermopower in two-dimensional graphene. Phys. Rev. B 2009, 80, 235415. (16) Small, J. P.; Perez, K. M.; Kim, P. Modulation of thermoelectric power of individual carbon nanotubes. Phys. Rev. Lett. 2003, 91, 256801. (17) Wu, X.; Hu, Y.; Ruan, M.; Madiomanana, N. K.; Berger, C.; de Heer, W. A. Thermoelectric effect in high mobility single layer epitaxial graphene. Appl. Phys. Lett. 2011, 99, 133102. (18) Wei, P.; Bao, W.; Pu, Y.; Lau, C. N.; Shi, J. Anomalous thermoelectric transport of Dirac particles in graphene. Phys. Rev. Lett. 2009, 102, 166808. (19) Checkelsky, J. G.; Ong, N. P. Thermopower and Nernst effect in graphene in a magnetic field. Phys. Rev. B 2009, 80, 081413. (20) Butch, N. P.; Kirshenbaum, K.; Syers, P.; Sushkov, A. B.; Jenkins, G. S.; Drew, H. D.; Paglione, J. Strong surface scattering in ultrahigh-mobility Bi2Se3 topological insulator crystals. Phys. Rev. B 2010, 81, 241301. (21) Kong, D.; Cha, J.; Lai, K.; Peng, H.; Analytis, J. G.; Meister, S.; Chen, Y.; Zhang, H. J.; Fisher, I. R.; Shen, Z. X.; Cui, Y. Rapid Surface 1706

dx.doi.org/10.1021/nl4032154 | Nano Lett. 2014, 14, 1701−1706